# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_KFe3Se2O6F6
_database_code_depnum_ccdc_archive 'CCDC 2086420'
loop_
_audit_author_name
_audit_author_address
'Minfeng Lu'
;Jiangsu University of Science and Technology
China
;
_audit_update_record             
;
2021-05-31 deposited with the CCDC.	2022-01-05 downloaded from the CCDC.
;
#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'F6 Fe3 K1 O6 Se2'
_chemical_formula_weight         574.5
_chemical_melting_point          ?
_chemical_compound_source        ?
_chemical_absolute_configuration .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting           trigonal
_symmetry_space_group_name_H-M   'P -3 m 1'
_symmetry_space_group_name_Hall  '-P 3;-2"'
_symmetry_Int_Tables_number      164

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -y,x-y,z
3 -x+y,-x,z
4 y,x,-z
5 x-y,-y,-z
6 -x,-x+y,-z
7 -x,-y,-z
8 y,-x+y,-z
9 x-y,x,-z
10 -y,-x,z
11 -x+y,y,z
12 x,x-y,z

_cell_length_a                   5.4261(2)
_cell_length_b                   5.4261(2)
_cell_length_c                   9.9929(4)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     254.799(17)

loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z            1

_cell_measurement_reflns_used    396
_cell_measurement_theta_min      2.086
_cell_measurement_theta_max      32.34
_cell_measurement_temperature    293
_cell_special_details            
; ?
;

_exptl_crystal_density_diffrn    3.7443
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             267

_exptl_absorpt_coefficient_mu    11.87
_exptl_crystal_description       transparent
_exptl_crystal_size_max          0.086
_exptl_crystal_size_mid          0.026
_exptl_crystal_size_min          0.023
_exptl_crystal_size_rad          ?
_exptl_crystal_colour            grey
_exptl_absorpt_correction_type   multi-scan'
_exptl_absorpt_process_details   Bruker
_exptl_absorpt_correction_T_min  0.5678
_exptl_absorpt_correction_T_max  0.7457
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           ?

_diffrn_ambient_temperature      293
_diffrn_source                   ?
_diffrn_source_power             ?
_diffrn_source_voltage           ?
_diffrn_source_current           ?
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device       CCD
_diffrn_measurement_device_type  'Bruker SMART BREEZE'
_diffrn_detector                 ?
_diffrn_detector_area_resol_mean ?
_diffrn_measurement_method       ?
_diffrn_measurement_specimen_support ?

_diffrn_reflns_number            3400
_diffrn_reflns_theta_min         2.04
_diffrn_reflns_theta_max         28.27
_diffrn_reflns_theta_full        28.27
_diffrn_measured_fraction_theta_max 1
_diffrn_measured_fraction_theta_full 1
_diffrn_reflns_av_R_equivalents  0.0495
_diffrn_reflns_av_unetI/netI     0.0183
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_reduction_process ?

_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?

_diffrn_radiation_probe          X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

_reflns_number_total             288
_reflns_number_gt                246
_reflns_threshold_expression     I>3σ(I)

_refine_ls_structure_factor_coef F
_refine_ls_R_factor_gt           0.0337
_refine_ls_wR_factor_gt          0.0420
_refine_ls_R_factor_all          0.0457
_refine_ls_wR_factor_ref         0.0432
_refine_ls_goodness_of_fit_ref   2.32
_refine_ls_goodness_of_fit_gt    2.46
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_reflns         288
_refine_ls_number_parameters     17
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0047
_refine_ls_shift/su_mean         0.0008
_refine_diff_density_max         1.27
_refine_diff_density_min         -1.27
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_abs_structure_details ?
_refine_ls_abs_structure_Flack   ?
_refine_ls_abs_structure_Rogers  ?

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
F 0.0171 0.0103 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Fe 0.3463 0.8444 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
K 0.2009 0.2494 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Mn 0.3368 0.7283 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0106 0.0060 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Se -0.0929 2.2259 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  ?
_computing_molecular_graphics    ?
_computing_publication_material  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?

loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?

loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?

loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
K1 K 0 0 0.5 Uani 0.0360(12) 1 1 d . . .
Fe1 Fe 0.333333 0.666667 0.23621(13) Uani 0.0075(4) 2 1 d . . .
Fe2 Fe 0 0 0 Uani 0.0052(5) 1 1 d . . .
Se1 Se 0.666667 0.333333 0.25824(9) Uani 0.0083(3) 2 1 d . . .
F1 F 0.1663(3) 0.3327(7) 0.1113(3) Uiso 0.0190(8) 6 1 d . . .
O1 O 0.5077(5) 0.4923(5) 0.3387(4) Uiso 0.0182(9) 6 1 d . . .


loop_
_jana_atom_site_ADP_C_label
_jana_atom_site_ADP_C_type_symbol
_jana_atom_site_ADP_C_111
_jana_atom_site_ADP_C_112
_jana_atom_site_ADP_C_113
_jana_atom_site_ADP_C_122
_jana_atom_site_ADP_C_123
_jana_atom_site_ADP_C_133
_jana_atom_site_ADP_C_222
_jana_atom_site_ADP_C_223
_jana_atom_site_ADP_C_233
_jana_atom_site_ADP_C_333
? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_D_label
_jana_atom_site_ADP_D_type_symbol
_jana_atom_site_ADP_D_1111
_jana_atom_site_ADP_D_1112
_jana_atom_site_ADP_D_1113
_jana_atom_site_ADP_D_1122
_jana_atom_site_ADP_D_1123
_jana_atom_site_ADP_D_1133
_jana_atom_site_ADP_D_1222
_jana_atom_site_ADP_D_1223
_jana_atom_site_ADP_D_1233
_jana_atom_site_ADP_D_1333
_jana_atom_site_ADP_D_2222
_jana_atom_site_ADP_D_2223
_jana_atom_site_ADP_D_2233
_jana_atom_site_ADP_D_2333
_jana_atom_site_ADP_D_3333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_E_label
_jana_atom_site_ADP_E_type_symbol
_jana_atom_site_ADP_E_11111
_jana_atom_site_ADP_E_11112
_jana_atom_site_ADP_E_11113
_jana_atom_site_ADP_E_11122
_jana_atom_site_ADP_E_11123
_jana_atom_site_ADP_E_11133
_jana_atom_site_ADP_E_11222
_jana_atom_site_ADP_E_11223
_jana_atom_site_ADP_E_11233
_jana_atom_site_ADP_E_11333
_jana_atom_site_ADP_E_12222
_jana_atom_site_ADP_E_12223
_jana_atom_site_ADP_E_12233
_jana_atom_site_ADP_E_12333
_jana_atom_site_ADP_E_13333
_jana_atom_site_ADP_E_22222
_jana_atom_site_ADP_E_22223
_jana_atom_site_ADP_E_22233
_jana_atom_site_ADP_E_22333
_jana_atom_site_ADP_E_23333
_jana_atom_site_ADP_E_33333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_F_label
_jana_atom_site_ADP_F_type_symbol
_jana_atom_site_ADP_F_111111
_jana_atom_site_ADP_F_111112
_jana_atom_site_ADP_F_111113
_jana_atom_site_ADP_F_111122
_jana_atom_site_ADP_F_111123
_jana_atom_site_ADP_F_111133
_jana_atom_site_ADP_F_111222
_jana_atom_site_ADP_F_111223
_jana_atom_site_ADP_F_111233
_jana_atom_site_ADP_F_111333
_jana_atom_site_ADP_F_112222
_jana_atom_site_ADP_F_112223
_jana_atom_site_ADP_F_112233
_jana_atom_site_ADP_F_112333
_jana_atom_site_ADP_F_113333
_jana_atom_site_ADP_F_122222
_jana_atom_site_ADP_F_122223
_jana_atom_site_ADP_F_122233
_jana_atom_site_ADP_F_122333
_jana_atom_site_ADP_F_123333
_jana_atom_site_ADP_F_133333
_jana_atom_site_ADP_F_222222
_jana_atom_site_ADP_F_222223
_jana_atom_site_ADP_F_222233
_jana_atom_site_ADP_F_222333
_jana_atom_site_ADP_F_223333
_jana_atom_site_ADP_F_233333
_jana_atom_site_ADP_F_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
K1 K1 . 1_445 5.4261(6) ?
K1 K1 . 1_455 5.4261(4) ?
K1 K1 . 1_545 5.4261(4) ?
K1 K1 . 1_565 5.4261(4) ?
K1 K1 . 1_655 5.4261(4) ?
K1 K1 . 1_665 5.4261(6) ?
K1 Fe1 . 1_445 4.0942(9) ?
K1 Fe1 . 1_545 4.0942(9) ?
K1 Fe1 . . 4.0942(9) ?
K1 Fe1 . 4_446 4.0942(9) ?
K1 Fe1 . 4_456 4.0942(9) ?
K1 Fe1 . 4_556 4.0942(9) ?
K1 Se1 . 1_445 3.9561(6) ?
K1 Se1 . 1_455 3.9561(6) ?
K1 Se1 . . 3.9561(6) ?
K1 Se1 . 4_446 3.9561(6) ?
K1 Se1 . 4_546 3.9561(6) ?
K1 Se1 . 4_556 3.9561(6) ?
K1 O1 . 1_445 3.156(3) ?
K1 O1 . . 3.156(3) ?
K1 O1 . 2_555 3.156(3) ?
K1 O1 . 2_655 3.156(3) ?
K1 O1 . 3_555 3.156(3) ?
K1 O1 . 3_565 3.156(3) ?
K1 O1 . 4_446 3.156(3) ?
K1 O1 . 4_556 3.156(3) ?
K1 O1 . 5_556 3.156(3) ?
K1 O1 . 5_566 3.156(3) ?
K1 O1 . 6_556 3.156(3) ?
K1 O1 . 6_656 3.156(3) ?
Fe1 F1 . . 2.005(3) ?
Fe1 F1 . 2_665 2.005(3) ?
Fe1 F1 . 3_565 2.005(4) ?
Fe1 O1 . . 1.933(3) ?
Fe1 O1 . 2_665 1.933(3) ?
Fe1 O1 . 3_565 1.933(3) ?
Fe2 F1 . . 1.919(3) ?
Fe2 F1 . 2_555 1.919(3) ?
Fe2 F1 . 3_555 1.919(4) ?
Fe2 F1 . 4_555 1.919(3) ?
Fe2 F1 . 5_555 1.919(3) ?
Fe2 F1 . 6_555 1.919(4) ?
Se1 O1 . . 1.697(3) ?
Se1 O1 . 2_655 1.697(3) ?
Se1 O1 . 3_665 1.697(3) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
K1 K1 K1 1_445 . 1_455 60.000(3) ?
K1 K1 K1 1_445 . 1_545 60.000(3) ?
K1 K1 K1 1_445 . 1_565 120.000(3) ?
K1 K1 K1 1_445 . 1_655 120.000(3) ?
K1 K1 K1 1_445 . 1_665 180.0(5) ?
K1 K1 Fe1 1_445 . 1_445 48.498(11) ?
K1 K1 Fe1 1_445 . 1_545 90.000(3) ?
K1 K1 Fe1 1_445 . . 131.502(11) ?
K1 K1 Fe1 1_445 . 4_446 48.498(11) ?
K1 K1 Fe1 1_445 . 4_456 90.000(3) ?
K1 K1 Fe1 1_445 . 4_556 131.502(11) ?
K1 K1 Se1 1_445 . 1_445 46.703(8) ?
K1 K1 Se1 1_445 . 1_455 90.000(3) ?
K1 K1 Se1 1_445 . . 133.297(8) ?
K1 K1 Se1 1_445 . 4_446 46.703(8) ?
K1 K1 Se1 1_445 . 4_546 90.000(3) ?
K1 K1 Se1 1_445 . 4_556 133.297(8) ?
K1 K1 O1 1_445 . 1_445 30.74(7) ?
K1 K1 O1 1_445 . . 149.26(7) ?
K1 K1 O1 1_445 . 2_555 65.80(5) ?
K1 K1 O1 1_445 . 2_655 116.72(5) ?
K1 K1 O1 1_445 . 3_555 63.28(5) ?
K1 K1 O1 1_445 . 3_565 114.20(5) ?
K1 K1 O1 1_445 . 4_446 30.74(7) ?
K1 K1 O1 1_445 . 4_556 149.26(7) ?
K1 K1 O1 1_445 . 5_556 65.80(5) ?
K1 K1 O1 1_445 . 5_566 116.72(5) ?
K1 K1 O1 1_445 . 6_556 63.28(5) ?
K1 K1 O1 1_445 . 6_656 114.20(5) ?
K1 K1 K1 1_455 . 1_545 120.000(2) ?
K1 K1 K1 1_455 . 1_565 60.000(2) ?
K1 K1 K1 1_455 . 1_655 180.0(5) ?
K1 K1 K1 1_455 . 1_665 120.000(3) ?
K1 K1 Fe1 1_455 . 1_445 48.498(11) ?
K1 K1 Fe1 1_455 . 1_545 131.502(11) ?
K1 K1 Fe1 1_455 . . 90.000(2) ?
K1 K1 Fe1 1_455 . 4_446 90.000(2) ?
K1 K1 Fe1 1_455 . 4_456 48.498(11) ?
K1 K1 Fe1 1_455 . 4_556 131.502(11) ?
K1 K1 Se1 1_455 . 1_445 90.000(2) ?
K1 K1 Se1 1_455 . 1_455 46.703(8) ?
K1 K1 Se1 1_455 . . 133.297(8) ?
K1 K1 Se1 1_455 . 4_446 46.703(8) ?
K1 K1 Se1 1_455 . 4_546 133.297(8) ?
K1 K1 Se1 1_455 . 4_556 90.000(2) ?
K1 K1 O1 1_455 . 1_445 65.80(6) ?
K1 K1 O1 1_455 . . 116.72(6) ?
K1 K1 O1 1_455 . 2_555 30.74(7) ?
K1 K1 O1 1_455 . 2_655 149.26(7) ?
K1 K1 O1 1_455 . 3_555 114.20(6) ?
K1 K1 O1 1_455 . 3_565 63.28(6) ?
K1 K1 O1 1_455 . 4_446 63.28(6) ?
K1 K1 O1 1_455 . 4_556 114.20(6) ?
K1 K1 O1 1_455 . 5_556 116.72(6) ?
K1 K1 O1 1_455 . 5_566 65.80(6) ?
K1 K1 O1 1_455 . 6_556 30.74(7) ?
K1 K1 O1 1_455 . 6_656 149.26(7) ?
K1 K1 K1 1_545 . 1_565 180.0(5) ?
K1 K1 K1 1_545 . 1_655 60.000(2) ?
K1 K1 K1 1_545 . 1_665 120.000(3) ?
K1 K1 Fe1 1_545 . 1_445 90.000(2) ?
K1 K1 Fe1 1_545 . 1_545 48.498(11) ?
K1 K1 Fe1 1_545 . . 131.502(11) ?
K1 K1 Fe1 1_545 . 4_446 48.498(11) ?
K1 K1 Fe1 1_545 . 4_456 131.502(11) ?
K1 K1 Fe1 1_545 . 4_556 90.000(2) ?
K1 K1 Se1 1_545 . 1_445 46.703(8) ?
K1 K1 Se1 1_545 . 1_455 133.297(8) ?
K1 K1 Se1 1_545 . . 90.000(2) ?
K1 K1 Se1 1_545 . 4_446 90.000(2) ?
K1 K1 Se1 1_545 . 4_546 46.703(8) ?
K1 K1 Se1 1_545 . 4_556 133.297(8) ?
K1 K1 O1 1_545 . 1_445 63.28(6) ?
K1 K1 O1 1_545 . . 114.20(6) ?
K1 K1 O1 1_545 . 2_555 116.72(6) ?
K1 K1 O1 1_545 . 2_655 65.80(6) ?
K1 K1 O1 1_545 . 3_555 30.74(7) ?
K1 K1 O1 1_545 . 3_565 149.26(7) ?
K1 K1 O1 1_545 . 4_446 65.80(6) ?
K1 K1 O1 1_545 . 4_556 116.72(6) ?
K1 K1 O1 1_545 . 5_556 30.74(7) ?
K1 K1 O1 1_545 . 5_566 149.26(7) ?
K1 K1 O1 1_545 . 6_556 114.20(6) ?
K1 K1 O1 1_545 . 6_656 63.28(6) ?
K1 K1 K1 1_565 . 1_655 120.000(2) ?
K1 K1 K1 1_565 . 1_665 60.000(3) ?
K1 K1 Fe1 1_565 . 1_445 90.000(2) ?
K1 K1 Fe1 1_565 . 1_545 131.502(11) ?
K1 K1 Fe1 1_565 . . 48.498(11) ?
K1 K1 Fe1 1_565 . 4_446 131.502(11) ?
K1 K1 Fe1 1_565 . 4_456 48.498(11) ?
K1 K1 Fe1 1_565 . 4_556 90.000(2) ?
K1 K1 Se1 1_565 . 1_445 133.297(8) ?
K1 K1 Se1 1_565 . 1_455 46.703(8) ?
K1 K1 Se1 1_565 . . 90.000(2) ?
K1 K1 Se1 1_565 . 4_446 90.000(2) ?
K1 K1 Se1 1_565 . 4_546 133.297(8) ?
K1 K1 Se1 1_565 . 4_556 46.703(8) ?
K1 K1 O1 1_565 . 1_445 116.72(6) ?
K1 K1 O1 1_565 . . 65.80(6) ?
K1 K1 O1 1_565 . 2_555 63.28(6) ?
K1 K1 O1 1_565 . 2_655 114.20(6) ?
K1 K1 O1 1_565 . 3_555 149.26(7) ?
K1 K1 O1 1_565 . 3_565 30.74(7) ?
K1 K1 O1 1_565 . 4_446 114.20(6) ?
K1 K1 O1 1_565 . 4_556 63.28(6) ?
K1 K1 O1 1_565 . 5_556 149.26(7) ?
K1 K1 O1 1_565 . 5_566 30.74(7) ?
K1 K1 O1 1_565 . 6_556 65.80(6) ?
K1 K1 O1 1_565 . 6_656 116.72(6) ?
K1 K1 K1 1_655 . 1_665 60.000(3) ?
K1 K1 Fe1 1_655 . 1_445 131.502(11) ?
K1 K1 Fe1 1_655 . 1_545 48.498(11) ?
K1 K1 Fe1 1_655 . . 90.000(2) ?
K1 K1 Fe1 1_655 . 4_446 90.000(2) ?
K1 K1 Fe1 1_655 . 4_456 131.502(11) ?
K1 K1 Fe1 1_655 . 4_556 48.498(11) ?
K1 K1 Se1 1_655 . 1_445 90.000(2) ?
K1 K1 Se1 1_655 . 1_455 133.297(8) ?
K1 K1 Se1 1_655 . . 46.703(8) ?
K1 K1 Se1 1_655 . 4_446 133.297(8) ?
K1 K1 Se1 1_655 . 4_546 46.703(8) ?
K1 K1 Se1 1_655 . 4_556 90.000(2) ?
K1 K1 O1 1_655 . 1_445 114.20(6) ?
K1 K1 O1 1_655 . . 63.28(6) ?
K1 K1 O1 1_655 . 2_555 149.26(7) ?
K1 K1 O1 1_655 . 2_655 30.74(7) ?
K1 K1 O1 1_655 . 3_555 65.80(6) ?
K1 K1 O1 1_655 . 3_565 116.72(6) ?
K1 K1 O1 1_655 . 4_446 116.72(6) ?
K1 K1 O1 1_655 . 4_556 65.80(6) ?
K1 K1 O1 1_655 . 5_556 63.28(6) ?
K1 K1 O1 1_655 . 5_566 114.20(6) ?
K1 K1 O1 1_655 . 6_556 149.26(7) ?
K1 K1 O1 1_655 . 6_656 30.74(7) ?
K1 K1 Fe1 1_665 . 1_445 131.502(11) ?
K1 K1 Fe1 1_665 . 1_545 90.000(3) ?
K1 K1 Fe1 1_665 . . 48.498(11) ?
K1 K1 Fe1 1_665 . 4_446 131.502(11) ?
K1 K1 Fe1 1_665 . 4_456 90.000(3) ?
K1 K1 Fe1 1_665 . 4_556 48.498(11) ?
K1 K1 Se1 1_665 . 1_445 133.297(8) ?
K1 K1 Se1 1_665 . 1_455 90.000(3) ?
K1 K1 Se1 1_665 . . 46.703(8) ?
K1 K1 Se1 1_665 . 4_446 133.297(8) ?
K1 K1 Se1 1_665 . 4_546 90.000(3) ?
K1 K1 Se1 1_665 . 4_556 46.703(8) ?
K1 K1 O1 1_665 . 1_445 149.26(7) ?
K1 K1 O1 1_665 . . 30.74(7) ?
K1 K1 O1 1_665 . 2_555 114.20(5) ?
K1 K1 O1 1_665 . 2_655 63.28(5) ?
K1 K1 O1 1_665 . 3_555 116.72(5) ?
K1 K1 O1 1_665 . 3_565 65.80(5) ?
K1 K1 O1 1_665 . 4_446 149.26(7) ?
K1 K1 O1 1_665 . 4_556 30.74(7) ?
K1 K1 O1 1_665 . 5_556 114.20(5) ?
K1 K1 O1 1_665 . 5_566 63.28(5) ?
K1 K1 O1 1_665 . 6_556 116.72(5) ?
K1 K1 O1 1_665 . 6_656 65.80(5) ?
Fe1 K1 Fe1 1_445 . 1_545 83.005(15) ?
Fe1 K1 Fe1 1_445 . . 83.005(15) ?
Fe1 K1 Fe1 1_445 . 4_446 96.995(15) ?
Fe1 K1 Fe1 1_445 . 4_456 96.995(15) ?
Fe1 K1 Fe1 1_445 . 4_556 180.0(5) ?
Fe1 K1 Se1 1_445 . 1_445 45.882(6) ?
Fe1 K1 Se1 1_445 . 1_455 45.882(6) ?
Fe1 K1 Se1 1_445 . . 102.283(18) ?
Fe1 K1 Se1 1_445 . 4_446 77.717(18) ?
Fe1 K1 Se1 1_445 . 4_546 134.118(6) ?
Fe1 K1 Se1 1_445 . 4_556 134.118(6) ?
Fe1 K1 O1 1_445 . 1_445 27.19(6) ?
Fe1 K1 O1 1_445 . . 104.46(7) ?
Fe1 K1 O1 1_445 . 2_555 27.19(6) ?
Fe1 K1 O1 1_445 . 2_655 104.46(6) ?
Fe1 K1 O1 1_445 . 3_555 69.74(7) ?
Fe1 K1 O1 1_445 . 3_565 69.74(5) ?
Fe1 K1 O1 1_445 . 4_446 75.54(7) ?
Fe1 K1 O1 1_445 . 4_556 152.81(6) ?
Fe1 K1 O1 1_445 . 5_556 110.26(5) ?
Fe1 K1 O1 1_445 . 5_566 110.26(7) ?
Fe1 K1 O1 1_445 . 6_556 75.54(6) ?
Fe1 K1 O1 1_445 . 6_656 152.81(6) ?
Fe1 K1 Fe1 1_545 . . 83.005(15) ?
Fe1 K1 Fe1 1_545 . 4_446 96.995(15) ?
Fe1 K1 Fe1 1_545 . 4_456 180.0(5) ?
Fe1 K1 Fe1 1_545 . 4_556 96.995(15) ?
Fe1 K1 Se1 1_545 . 1_445 45.882(6) ?
Fe1 K1 Se1 1_545 . 1_455 102.283(18) ?
Fe1 K1 Se1 1_545 . . 45.882(6) ?
Fe1 K1 Se1 1_545 . 4_446 134.118(6) ?
Fe1 K1 Se1 1_545 . 4_546 77.717(18) ?
Fe1 K1 Se1 1_545 . 4_556 134.118(6) ?
Fe1 K1 O1 1_545 . 1_445 69.74(6) ?
Fe1 K1 O1 1_545 . . 69.74(6) ?
Fe1 K1 O1 1_545 . 2_555 104.46(7) ?
Fe1 K1 O1 1_545 . 2_655 27.19(5) ?
Fe1 K1 O1 1_545 . 3_555 27.19(5) ?
Fe1 K1 O1 1_545 . 3_565 104.46(7) ?
Fe1 K1 O1 1_545 . 4_446 110.26(6) ?
Fe1 K1 O1 1_545 . 4_556 110.26(6) ?
Fe1 K1 O1 1_545 . 5_556 75.54(7) ?
Fe1 K1 O1 1_545 . 5_566 152.81(5) ?
Fe1 K1 O1 1_545 . 6_556 152.81(5) ?
Fe1 K1 O1 1_545 . 6_656 75.54(7) ?
Fe1 K1 Fe1 . . 4_446 180.0(5) ?
Fe1 K1 Fe1 . . 4_456 96.995(15) ?
Fe1 K1 Fe1 . . 4_556 96.995(15) ?
Fe1 K1 Se1 . . 1_445 102.283(18) ?
Fe1 K1 Se1 . . 1_455 45.882(6) ?
Fe1 K1 Se1 . . . 45.882(6) ?
Fe1 K1 Se1 . . 4_446 134.118(6) ?
Fe1 K1 Se1 . . 4_546 134.118(6) ?
Fe1 K1 Se1 . . 4_556 77.717(18) ?
Fe1 K1 O1 . . 1_445 104.46(7) ?
Fe1 K1 O1 . . . 27.19(6) ?
Fe1 K1 O1 . . 2_555 69.74(5) ?
Fe1 K1 O1 . . 2_655 69.74(7) ?
Fe1 K1 O1 . . 3_555 104.46(6) ?
Fe1 K1 O1 . . 3_565 27.19(6) ?
Fe1 K1 O1 . . 4_446 152.81(6) ?
Fe1 K1 O1 . . 4_556 75.54(7) ?
Fe1 K1 O1 . . 5_556 152.81(6) ?
Fe1 K1 O1 . . 5_566 75.54(6) ?
Fe1 K1 O1 . . 6_556 110.26(7) ?
Fe1 K1 O1 . . 6_656 110.26(5) ?
Fe1 K1 Fe1 4_446 . 4_456 83.005(15) ?
Fe1 K1 Fe1 4_446 . 4_556 83.005(15) ?
Fe1 K1 Se1 4_446 . 1_445 77.717(18) ?
Fe1 K1 Se1 4_446 . 1_455 134.118(6) ?
Fe1 K1 Se1 4_446 . . 134.118(6) ?
Fe1 K1 Se1 4_446 . 4_446 45.882(6) ?
Fe1 K1 Se1 4_446 . 4_546 45.882(6) ?
Fe1 K1 Se1 4_446 . 4_556 102.283(18) ?
Fe1 K1 O1 4_446 . 1_445 75.54(7) ?
Fe1 K1 O1 4_446 . . 152.81(6) ?
Fe1 K1 O1 4_446 . 2_555 110.26(5) ?
Fe1 K1 O1 4_446 . 2_655 110.26(7) ?
Fe1 K1 O1 4_446 . 3_555 75.54(6) ?
Fe1 K1 O1 4_446 . 3_565 152.81(6) ?
Fe1 K1 O1 4_446 . 4_446 27.19(6) ?
Fe1 K1 O1 4_446 . 4_556 104.46(7) ?
Fe1 K1 O1 4_446 . 5_556 27.19(6) ?
Fe1 K1 O1 4_446 . 5_566 104.46(6) ?
Fe1 K1 O1 4_446 . 6_556 69.74(7) ?
Fe1 K1 O1 4_446 . 6_656 69.74(5) ?
Fe1 K1 Fe1 4_456 . 4_556 83.005(15) ?
Fe1 K1 Se1 4_456 . 1_445 134.118(6) ?
Fe1 K1 Se1 4_456 . 1_455 77.717(18) ?
Fe1 K1 Se1 4_456 . . 134.118(6) ?
Fe1 K1 Se1 4_456 . 4_446 45.882(6) ?
Fe1 K1 Se1 4_456 . 4_546 102.283(18) ?
Fe1 K1 Se1 4_456 . 4_556 45.882(6) ?
Fe1 K1 O1 4_456 . 1_445 110.26(6) ?
Fe1 K1 O1 4_456 . . 110.26(6) ?
Fe1 K1 O1 4_456 . 2_555 75.54(7) ?
Fe1 K1 O1 4_456 . 2_655 152.81(5) ?
Fe1 K1 O1 4_456 . 3_555 152.81(5) ?
Fe1 K1 O1 4_456 . 3_565 75.54(7) ?
Fe1 K1 O1 4_456 . 4_446 69.74(6) ?
Fe1 K1 O1 4_456 . 4_556 69.74(6) ?
Fe1 K1 O1 4_456 . 5_556 104.46(7) ?
Fe1 K1 O1 4_456 . 5_566 27.19(5) ?
Fe1 K1 O1 4_456 . 6_556 27.19(5) ?
Fe1 K1 O1 4_456 . 6_656 104.46(7) ?
Fe1 K1 Se1 4_556 . 1_445 134.118(6) ?
Fe1 K1 Se1 4_556 . 1_455 134.118(6) ?
Fe1 K1 Se1 4_556 . . 77.717(18) ?
Fe1 K1 Se1 4_556 . 4_446 102.283(18) ?
Fe1 K1 Se1 4_556 . 4_546 45.882(6) ?
Fe1 K1 Se1 4_556 . 4_556 45.882(6) ?
Fe1 K1 O1 4_556 . 1_445 152.81(6) ?
Fe1 K1 O1 4_556 . . 75.54(7) ?
Fe1 K1 O1 4_556 . 2_555 152.81(6) ?
Fe1 K1 O1 4_556 . 2_655 75.54(6) ?
Fe1 K1 O1 4_556 . 3_555 110.26(7) ?
Fe1 K1 O1 4_556 . 3_565 110.26(5) ?
Fe1 K1 O1 4_556 . 4_446 104.46(7) ?
Fe1 K1 O1 4_556 . 4_556 27.19(6) ?
Fe1 K1 O1 4_556 . 5_556 69.74(5) ?
Fe1 K1 O1 4_556 . 5_566 69.74(7) ?
Fe1 K1 O1 4_556 . 6_556 104.46(6) ?
Fe1 K1 O1 4_556 . 6_656 27.19(6) ?
Se1 K1 Se1 1_445 . 1_455 86.595(11) ?
Se1 K1 Se1 1_445 . . 86.595(11) ?
Se1 K1 Se1 1_445 . 4_446 93.405(11) ?
Se1 K1 Se1 1_445 . 4_546 93.405(11) ?
Se1 K1 Se1 1_445 . 4_556 180.0(5) ?
Se1 K1 O1 1_445 . 1_445 24.45(6) ?
Se1 K1 O1 1_445 . . 105.58(6) ?
Se1 K1 O1 1_445 . 2_555 72.92(7) ?
Se1 K1 O1 1_445 . 2_655 72.92(5) ?
Se1 K1 O1 1_445 . 3_555 24.45(6) ?
Se1 K1 O1 1_445 . 3_565 105.58(6) ?
Se1 K1 O1 1_445 . 4_446 74.42(6) ?
Se1 K1 O1 1_445 . 4_556 155.55(6) ?
Se1 K1 O1 1_445 . 5_556 74.42(6) ?
Se1 K1 O1 1_445 . 5_566 155.55(6) ?
Se1 K1 O1 1_445 . 6_556 107.08(5) ?
Se1 K1 O1 1_445 . 6_656 107.08(7) ?
Se1 K1 Se1 1_455 . . 86.595(11) ?
Se1 K1 Se1 1_455 . 4_446 93.405(11) ?
Se1 K1 Se1 1_455 . 4_546 180.0(5) ?
Se1 K1 Se1 1_455 . 4_556 93.405(11) ?
Se1 K1 O1 1_455 . 1_445 72.92(6) ?
Se1 K1 O1 1_455 . . 72.92(6) ?
Se1 K1 O1 1_455 . 2_555 24.45(5) ?
Se1 K1 O1 1_455 . 2_655 105.58(7) ?
Se1 K1 O1 1_455 . 3_555 105.58(7) ?
Se1 K1 O1 1_455 . 3_565 24.45(5) ?
Se1 K1 O1 1_455 . 4_446 107.08(6) ?
Se1 K1 O1 1_455 . 4_556 107.08(6) ?
Se1 K1 O1 1_455 . 5_556 155.55(5) ?
Se1 K1 O1 1_455 . 5_566 74.42(7) ?
Se1 K1 O1 1_455 . 6_556 74.42(7) ?
Se1 K1 O1 1_455 . 6_656 155.55(5) ?
Se1 K1 Se1 . . 4_446 180.0(5) ?
Se1 K1 Se1 . . 4_546 93.405(11) ?
Se1 K1 Se1 . . 4_556 93.405(11) ?
Se1 K1 O1 . . 1_445 105.58(6) ?
Se1 K1 O1 . . . 24.45(6) ?
Se1 K1 O1 . . 2_555 105.58(6) ?
Se1 K1 O1 . . 2_655 24.45(6) ?
Se1 K1 O1 . . 3_555 72.92(5) ?
Se1 K1 O1 . . 3_565 72.92(7) ?
Se1 K1 O1 . . 4_446 155.55(6) ?
Se1 K1 O1 . . 4_556 74.42(6) ?
Se1 K1 O1 . . 5_556 107.08(7) ?
Se1 K1 O1 . . 5_566 107.08(5) ?
Se1 K1 O1 . . 6_556 155.55(6) ?
Se1 K1 O1 . . 6_656 74.42(6) ?
Se1 K1 Se1 4_446 . 4_546 86.595(11) ?
Se1 K1 Se1 4_446 . 4_556 86.595(11) ?
Se1 K1 O1 4_446 . 1_445 74.42(6) ?
Se1 K1 O1 4_446 . . 155.55(6) ?
Se1 K1 O1 4_446 . 2_555 74.42(6) ?
Se1 K1 O1 4_446 . 2_655 155.55(6) ?
Se1 K1 O1 4_446 . 3_555 107.08(5) ?
Se1 K1 O1 4_446 . 3_565 107.08(7) ?
Se1 K1 O1 4_446 . 4_446 24.45(6) ?
Se1 K1 O1 4_446 . 4_556 105.58(6) ?
Se1 K1 O1 4_446 . 5_556 72.92(7) ?
Se1 K1 O1 4_446 . 5_566 72.92(5) ?
Se1 K1 O1 4_446 . 6_556 24.45(6) ?
Se1 K1 O1 4_446 . 6_656 105.58(6) ?
Se1 K1 Se1 4_546 . 4_556 86.595(11) ?
Se1 K1 O1 4_546 . 1_445 107.08(6) ?
Se1 K1 O1 4_546 . . 107.08(6) ?
Se1 K1 O1 4_546 . 2_555 155.55(5) ?
Se1 K1 O1 4_546 . 2_655 74.42(7) ?
Se1 K1 O1 4_546 . 3_555 74.42(7) ?
Se1 K1 O1 4_546 . 3_565 155.55(5) ?
Se1 K1 O1 4_546 . 4_446 72.92(6) ?
Se1 K1 O1 4_546 . 4_556 72.92(6) ?
Se1 K1 O1 4_546 . 5_556 24.45(5) ?
Se1 K1 O1 4_546 . 5_566 105.58(7) ?
Se1 K1 O1 4_546 . 6_556 105.58(7) ?
Se1 K1 O1 4_546 . 6_656 24.45(5) ?
Se1 K1 O1 4_556 . 1_445 155.55(6) ?
Se1 K1 O1 4_556 . . 74.42(6) ?
Se1 K1 O1 4_556 . 2_555 107.08(7) ?
Se1 K1 O1 4_556 . 2_655 107.08(5) ?
Se1 K1 O1 4_556 . 3_555 155.55(6) ?
Se1 K1 O1 4_556 . 3_565 74.42(6) ?
Se1 K1 O1 4_556 . 4_446 105.58(6) ?
Se1 K1 O1 4_556 . 4_556 24.45(6) ?
Se1 K1 O1 4_556 . 5_556 105.58(6) ?
Se1 K1 O1 4_556 . 5_566 24.45(6) ?
Se1 K1 O1 4_556 . 6_556 72.92(5) ?
Se1 K1 O1 4_556 . 6_656 72.92(7) ?
O1 K1 O1 1_445 . . 118.53(9) ?
O1 K1 O1 1_445 . 2_555 53.44(8) ?
O1 K1 O1 1_445 . 2_655 96.26(8) ?
O1 K1 O1 1_445 . 3_555 48.40(8) ?
O1 K1 O1 1_445 . 3_565 96.26(8) ?
O1 K1 O1 1_445 . 4_446 61.47(9) ?
O1 K1 O1 1_445 . 4_556 180.0(5) ?
O1 K1 O1 1_445 . 5_556 83.74(8) ?
O1 K1 O1 1_445 . 5_566 131.60(8) ?
O1 K1 O1 1_445 . 6_556 83.74(8) ?
O1 K1 O1 1_445 . 6_656 126.56(8) ?
O1 K1 O1 . . 2_555 96.26(8) ?
O1 K1 O1 . . 2_655 48.40(8) ?
O1 K1 O1 . . 3_555 96.26(8) ?
O1 K1 O1 . . 3_565 53.44(8) ?
O1 K1 O1 . . 4_446 180.0(5) ?
O1 K1 O1 . . 4_556 61.47(9) ?
O1 K1 O1 . . 5_556 126.56(8) ?
O1 K1 O1 . . 5_566 83.74(8) ?
O1 K1 O1 . . 6_556 131.60(8) ?
O1 K1 O1 . . 6_656 83.74(8) ?
O1 K1 O1 2_555 . 2_655 118.53(10) ?
O1 K1 O1 2_555 . 3_555 96.26(10) ?
O1 K1 O1 2_555 . 3_565 48.40(7) ?
O1 K1 O1 2_555 . 4_446 83.74(8) ?
O1 K1 O1 2_555 . 4_556 126.56(8) ?
O1 K1 O1 2_555 . 5_556 131.60(7) ?
O1 K1 O1 2_555 . 5_566 83.74(10) ?
O1 K1 O1 2_555 . 6_556 61.47(10) ?
O1 K1 O1 2_555 . 6_656 180.0(5) ?
O1 K1 O1 2_655 . 3_555 53.44(7) ?
O1 K1 O1 2_655 . 3_565 96.26(10) ?
O1 K1 O1 2_655 . 4_446 131.60(8) ?
O1 K1 O1 2_655 . 4_556 83.74(8) ?
O1 K1 O1 2_655 . 5_556 83.74(10) ?
O1 K1 O1 2_655 . 5_566 126.56(7) ?
O1 K1 O1 2_655 . 6_556 180.0(5) ?
O1 K1 O1 2_655 . 6_656 61.47(10) ?
O1 K1 O1 3_555 . 3_565 118.53(10) ?
O1 K1 O1 3_555 . 4_446 83.74(8) ?
O1 K1 O1 3_555 . 4_556 131.60(8) ?
O1 K1 O1 3_555 . 5_556 61.47(10) ?
O1 K1 O1 3_555 . 5_566 180.0(5) ?
O1 K1 O1 3_555 . 6_556 126.56(7) ?
O1 K1 O1 3_555 . 6_656 83.74(10) ?
O1 K1 O1 3_565 . 4_446 126.56(8) ?
O1 K1 O1 3_565 . 4_556 83.74(8) ?
O1 K1 O1 3_565 . 5_556 180.0(5) ?
O1 K1 O1 3_565 . 5_566 61.47(10) ?
O1 K1 O1 3_565 . 6_556 83.74(10) ?
O1 K1 O1 3_565 . 6_656 131.60(7) ?
O1 K1 O1 4_446 . 4_556 118.53(9) ?
O1 K1 O1 4_446 . 5_556 53.44(8) ?
O1 K1 O1 4_446 . 5_566 96.26(8) ?
O1 K1 O1 4_446 . 6_556 48.40(8) ?
O1 K1 O1 4_446 . 6_656 96.26(8) ?
O1 K1 O1 4_556 . 5_556 96.26(8) ?
O1 K1 O1 4_556 . 5_566 48.40(8) ?
O1 K1 O1 4_556 . 6_556 96.26(8) ?
O1 K1 O1 4_556 . 6_656 53.44(8) ?
O1 K1 O1 5_556 . 5_566 118.53(10) ?
O1 K1 O1 5_556 . 6_556 96.26(10) ?
O1 K1 O1 5_556 . 6_656 48.40(7) ?
O1 K1 O1 5_566 . 6_556 53.44(7) ?
O1 K1 O1 5_566 . 6_656 96.26(10) ?
O1 K1 O1 6_556 . 6_656 118.53(10) ?
K1 Fe1 K1 . . 1_565 83.00(2) ?
K1 Fe1 K1 . . 1_665 83.00(2) ?
K1 Fe1 F1 . . . 78.57(9) ?
K1 Fe1 F1 . . 2_665 134.44(13) ?
K1 Fe1 F1 . . 3_565 134.44(9) ?
K1 Fe1 O1 . . . 48.26(7) ?
K1 Fe1 O1 . . 2_665 107.91(12) ?
K1 Fe1 O1 . . 3_565 48.26(11) ?
K1 Fe1 K1 1_565 . 1_665 83.00(2) ?
K1 Fe1 F1 1_565 . . 134.44(6) ?
K1 Fe1 F1 1_565 . 2_665 134.44(12) ?
K1 Fe1 F1 1_565 . 3_565 78.57(10) ?
K1 Fe1 O1 1_565 . . 107.91(12) ?
K1 Fe1 O1 1_565 . 2_665 48.26(9) ?
K1 Fe1 O1 1_565 . 3_565 48.26(9) ?
K1 Fe1 F1 1_665 . . 134.44(9) ?
K1 Fe1 F1 1_665 . 2_665 78.57(9) ?
K1 Fe1 F1 1_665 . 3_565 134.44(5) ?
K1 Fe1 O1 1_665 . . 48.26(7) ?
K1 Fe1 O1 1_665 . 2_665 48.26(11) ?
K1 Fe1 O1 1_665 . 3_565 107.91(12) ?
F1 Fe1 F1 . . 2_665 85.35(12) ?
F1 Fe1 F1 . . 3_565 85.35(13) ?
F1 Fe1 O1 . . . 89.89(14) ?
F1 Fe1 O1 . . 2_665 173.52(16) ?
F1 Fe1 O1 . . 3_565 89.89(11) ?
F1 Fe1 F1 2_665 . 3_565 85.35(17) ?
F1 Fe1 O1 2_665 . . 89.89(16) ?
F1 Fe1 O1 2_665 . 2_665 89.89(14) ?
F1 Fe1 O1 2_665 . 3_565 173.52(16) ?
F1 Fe1 O1 3_565 . . 173.52(16) ?
F1 Fe1 O1 3_565 . 2_665 89.89(13) ?
F1 Fe1 O1 3_565 . 3_565 89.89(15) ?
O1 Fe1 O1 . . 2_665 94.50(15) ?
O1 Fe1 O1 . . 3_565 94.50(15) ?
O1 Fe1 O1 2_665 . 3_565 94.50(13) ?
F1 Fe2 F1 . . 2_555 89.76(12) ?
F1 Fe2 F1 . . 3_555 89.76(12) ?
F1 Fe2 F1 . . 4_555 90.24(10) ?
F1 Fe2 F1 . . 5_555 180.0(5) ?
F1 Fe2 F1 . . 6_555 90.24(15) ?
F1 Fe2 F1 2_555 . 3_555 89.76(17) ?
F1 Fe2 F1 2_555 . 4_555 180.0(5) ?
F1 Fe2 F1 2_555 . 5_555 90.24(15) ?
F1 Fe2 F1 2_555 . 6_555 90.24(15) ?
F1 Fe2 F1 3_555 . 4_555 90.24(15) ?
F1 Fe2 F1 3_555 . 5_555 90.24(15) ?
F1 Fe2 F1 3_555 . 6_555 180.0(5) ?
F1 Fe2 F1 4_555 . 5_555 89.76(12) ?
F1 Fe2 F1 4_555 . 6_555 89.76(12) ?
F1 Fe2 F1 5_555 . 6_555 89.76(17) ?
K1 Se1 K1 . . 1_655 86.595(16) ?
K1 Se1 K1 . . 1_665 86.595(16) ?
K1 Se1 O1 . . . 50.35(8) ?
K1 Se1 O1 . . 2_655 50.35(12) ?
K1 Se1 O1 . . 3_665 114.06(14) ?
K1 Se1 K1 1_655 . 1_665 86.595(16) ?
K1 Se1 O1 1_655 . . 114.06(14) ?
K1 Se1 O1 1_655 . 2_655 50.35(10) ?
K1 Se1 O1 1_655 . 3_665 50.35(10) ?
K1 Se1 O1 1_665 . . 50.35(8) ?
K1 Se1 O1 1_665 . 2_655 114.06(14) ?
K1 Se1 O1 1_665 . 3_665 50.35(12) ?
O1 Se1 O1 . . 2_655 99.37(16) ?
O1 Se1 O1 . . 3_665 99.37(16) ?
O1 Se1 O1 2_655 . 3_665 99.37(15) ?
Fe1 F1 Fe2 . . . 176.95(19) ?
K1 O1 K1 . . 1_665 118.53(13) ?
K1 O1 Fe1 . . . 104.55(9) ?
K1 O1 Se1 . . . 105.20(10) ?
K1 O1 Fe1 1_665 . . 104.55(9) ?
K1 O1 Se1 1_665 . . 105.20(10) ?
Fe1 O1 Se1 . . . 119.7(2) ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?


####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data__RbFe3Se2O6F6
_database_code_depnum_ccdc_archive 'CCDC 2086421'
loop_
_audit_author_name
_audit_author_address
'Minfeng Lu'
;Jiangsu University of Science and Technology
China
;
_audit_update_record             
;
2021-09-30 deposited with the CCDC.	2022-01-05 downloaded from the CCDC.
;
#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'F6 Fe3 O6 Rb1 Se2'
_chemical_formula_weight         620.9
_chemical_melting_point          ?
_chemical_compound_source        ?
_chemical_absolute_configuration .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting           trigonal
_symmetry_space_group_name_H-M   'P -3 m 1'
_symmetry_space_group_name_Hall  '-P 3;-2"'
_symmetry_Int_Tables_number      164

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -y,x-y,z
3 -x+y,-x,z
4 y,x,-z
5 x-y,-y,-z
6 -x,-x+y,-z
7 -x,-y,-z
8 y,-x+y,-z
9 x-y,x,-z
10 -y,-x,z
11 -x+y,y,z
12 x,x-y,z

_cell_length_a                   5.4478(2)
_cell_length_b                   5.4478(2)
_cell_length_c                   10.1584(3)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     261.095(16)

loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z            1

_cell_measurement_reflns_used    364
_cell_measurement_theta_min      1.996
_cell_measurement_theta_max      29.865
_cell_measurement_temperature    293
_cell_special_details            
; ?
;

_exptl_crystal_density_diffrn    3.9489
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             285

_exptl_absorpt_coefficient_mu    15.816
_exptl_crystal_description       transparent
_exptl_crystal_size_max          0.076
_exptl_crystal_size_mid          0.022
_exptl_crystal_size_min          0.019
_exptl_crystal_size_rad          ?
_exptl_crystal_colour            grey
_exptl_absorpt_correction_type   multi-scan'
_exptl_absorpt_process_details   Bruker
_exptl_absorpt_correction_T_min  0.4780
_exptl_absorpt_correction_T_max  0.7457
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           ?

_diffrn_ambient_temperature      293
_diffrn_source                   ?
_diffrn_source_power             ?
_diffrn_source_voltage           ?
_diffrn_source_current           ?
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device       CCD
_diffrn_measurement_device_type  'Bruker apex II'
_diffrn_detector                 ?
_diffrn_detector_area_resol_mean ?
_diffrn_measurement_method       ?
_diffrn_measurement_specimen_support ?

_diffrn_reflns_number            3543
_diffrn_reflns_theta_min         2
_diffrn_reflns_theta_max         28.24
_diffrn_reflns_theta_full        28.24
_diffrn_measured_fraction_theta_max 1
_diffrn_measured_fraction_theta_full 1
_diffrn_reflns_av_R_equivalents  0.0683
_diffrn_reflns_av_unetI/netI     0.026
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_reduction_process ?

_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?

_diffrn_radiation_probe          X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

_reflns_number_total             293
_reflns_number_gt                232
_reflns_threshold_expression     I>3σ(I)

_refine_ls_structure_factor_coef F
_refine_ls_R_factor_gt           0.0331
_refine_ls_wR_factor_gt          0.0350
_refine_ls_R_factor_all          0.0433
_refine_ls_wR_factor_ref         0.0362
_refine_ls_goodness_of_fit_ref   1.55
_refine_ls_goodness_of_fit_gt    1.70
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_reflns         293
_refine_ls_number_parameters     17
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0420
_refine_ls_shift/su_mean         0.0152
_refine_diff_density_max         0.71
_refine_diff_density_min         -1.03
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_abs_structure_details ?
_refine_ls_abs_structure_Flack   ?
_refine_ls_abs_structure_Rogers  ?

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
F 0.0171 0.0103 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Fe 0.3463 0.8444 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0106 0.0060 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Rb -0.9393 2.9676 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Se -0.0929 2.2259 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  ?
_computing_molecular_graphics    ?
_computing_publication_material  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?

loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?

loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?

loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Rb1 Rb 0 0 0.5 Uani 0.0236(5) 1 1 d . . .
Fe1 Fe 0.333333 0.666667 0.23188(11) Uani 0.0081(4) 2 1 d . . .
Fe2 Fe 0 0 0 Uani 0.0069(5) 1 1 d . . .
Se1 Se 0.666667 0.333333 0.25402(8) Uani 0.0099(3) 2 1 d . . .
F1 F 0.1664(4) 0.3329(7) 0.1088(3) Uiso 0.0183(8) 6 1 d . . .
O1 O 0.5074(5) 0.4926(5) 0.3329(3) Uiso 0.0130(9) 6 1 d . . .


loop_
_jana_atom_site_ADP_C_label
_jana_atom_site_ADP_C_type_symbol
_jana_atom_site_ADP_C_111
_jana_atom_site_ADP_C_112
_jana_atom_site_ADP_C_113
_jana_atom_site_ADP_C_122
_jana_atom_site_ADP_C_123
_jana_atom_site_ADP_C_133
_jana_atom_site_ADP_C_222
_jana_atom_site_ADP_C_223
_jana_atom_site_ADP_C_233
_jana_atom_site_ADP_C_333
? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_D_label
_jana_atom_site_ADP_D_type_symbol
_jana_atom_site_ADP_D_1111
_jana_atom_site_ADP_D_1112
_jana_atom_site_ADP_D_1113
_jana_atom_site_ADP_D_1122
_jana_atom_site_ADP_D_1123
_jana_atom_site_ADP_D_1133
_jana_atom_site_ADP_D_1222
_jana_atom_site_ADP_D_1223
_jana_atom_site_ADP_D_1233
_jana_atom_site_ADP_D_1333
_jana_atom_site_ADP_D_2222
_jana_atom_site_ADP_D_2223
_jana_atom_site_ADP_D_2233
_jana_atom_site_ADP_D_2333
_jana_atom_site_ADP_D_3333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_E_label
_jana_atom_site_ADP_E_type_symbol
_jana_atom_site_ADP_E_11111
_jana_atom_site_ADP_E_11112
_jana_atom_site_ADP_E_11113
_jana_atom_site_ADP_E_11122
_jana_atom_site_ADP_E_11123
_jana_atom_site_ADP_E_11133
_jana_atom_site_ADP_E_11222
_jana_atom_site_ADP_E_11223
_jana_atom_site_ADP_E_11233
_jana_atom_site_ADP_E_11333
_jana_atom_site_ADP_E_12222
_jana_atom_site_ADP_E_12223
_jana_atom_site_ADP_E_12233
_jana_atom_site_ADP_E_12333
_jana_atom_site_ADP_E_13333
_jana_atom_site_ADP_E_22222
_jana_atom_site_ADP_E_22223
_jana_atom_site_ADP_E_22233
_jana_atom_site_ADP_E_22333
_jana_atom_site_ADP_E_23333
_jana_atom_site_ADP_E_33333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_F_label
_jana_atom_site_ADP_F_type_symbol
_jana_atom_site_ADP_F_111111
_jana_atom_site_ADP_F_111112
_jana_atom_site_ADP_F_111113
_jana_atom_site_ADP_F_111122
_jana_atom_site_ADP_F_111123
_jana_atom_site_ADP_F_111133
_jana_atom_site_ADP_F_111222
_jana_atom_site_ADP_F_111223
_jana_atom_site_ADP_F_111233
_jana_atom_site_ADP_F_111333
_jana_atom_site_ADP_F_112222
_jana_atom_site_ADP_F_112223
_jana_atom_site_ADP_F_112233
_jana_atom_site_ADP_F_112333
_jana_atom_site_ADP_F_113333
_jana_atom_site_ADP_F_122222
_jana_atom_site_ADP_F_122223
_jana_atom_site_ADP_F_122233
_jana_atom_site_ADP_F_122333
_jana_atom_site_ADP_F_123333
_jana_atom_site_ADP_F_133333
_jana_atom_site_ADP_F_222222
_jana_atom_site_ADP_F_222223
_jana_atom_site_ADP_F_222233
_jana_atom_site_ADP_F_222333
_jana_atom_site_ADP_F_223333
_jana_atom_site_ADP_F_233333
_jana_atom_site_ADP_F_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Rb1 Rb1 . 1_445 5.4478(6) ?
Rb1 Rb1 . 1_455 5.4478(4) ?
Rb1 Rb1 . 1_545 5.4478(4) ?
Rb1 Rb1 . 1_565 5.4478(4) ?
Rb1 Rb1 . 1_655 5.4478(4) ?
Rb1 Rb1 . 1_665 5.4478(6) ?
Rb1 Fe1 . 1_445 4.1607(8) ?
Rb1 Fe1 . 1_545 4.1607(8) ?
Rb1 Fe1 . . 4.1607(8) ?
Rb1 Fe1 . 4_446 4.1607(8) ?
Rb1 Fe1 . 4_456 4.1607(8) ?
Rb1 Fe1 . 4_556 4.1607(8) ?
Rb1 Se1 . 1_445 4.0171(6) ?
Rb1 Se1 . 1_455 4.0171(5) ?
Rb1 Se1 . . 4.0171(6) ?
Rb1 Se1 . 4_446 4.0171(6) ?
Rb1 Se1 . 4_546 4.0171(5) ?
Rb1 Se1 . 4_556 4.0171(6) ?
Rb1 O1 . 1_445 3.210(2) ?
Rb1 O1 . . 3.210(2) ?
Rb1 O1 . 2_555 3.210(3) ?
Rb1 O1 . 2_655 3.210(3) ?
Rb1 O1 . 3_555 3.210(3) ?
Rb1 O1 . 3_565 3.210(3) ?
Rb1 O1 . 4_446 3.210(2) ?
Rb1 O1 . 4_556 3.210(2) ?
Rb1 O1 . 5_556 3.210(3) ?
Rb1 O1 . 5_566 3.210(3) ?
Rb1 O1 . 6_556 3.210(3) ?
Rb1 O1 . 6_656 3.210(3) ?
Fe1 F1 . . 2.011(3) ?
Fe1 F1 . 2_665 2.011(3) ?
Fe1 F1 . 3_565 2.011(4) ?
Fe1 O1 . . 1.937(3) ?
Fe1 O1 . 2_665 1.937(3) ?
Fe1 O1 . 3_565 1.937(3) ?
Fe2 F1 . . 1.920(3) ?
Fe2 F1 . 2_555 1.920(3) ?
Fe2 F1 . 3_555 1.920(4) ?
Fe2 F1 . 4_555 1.920(3) ?
Fe2 F1 . 5_555 1.920(3) ?
Fe2 F1 . 6_555 1.920(4) ?
Se1 O1 . . 1.703(3) ?
Se1 O1 . 2_655 1.703(3) ?
Se1 O1 . 3_665 1.703(3) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Rb1 Rb1 Rb1 1_445 . 1_455 60.000(3) ?
Rb1 Rb1 Rb1 1_445 . 1_545 60.000(3) ?
Rb1 Rb1 Rb1 1_445 . 1_565 120.000(3) ?
Rb1 Rb1 Rb1 1_445 . 1_655 120.000(3) ?
Rb1 Rb1 Rb1 1_445 . 1_665 180.0(5) ?
Rb1 Rb1 Fe1 1_445 . 1_445 49.105(9) ?
Rb1 Rb1 Fe1 1_445 . 1_545 90.000(3) ?
Rb1 Rb1 Fe1 1_445 . . 130.895(9) ?
Rb1 Rb1 Fe1 1_445 . 4_446 49.105(9) ?
Rb1 Rb1 Fe1 1_445 . 4_456 90.000(3) ?
Rb1 Rb1 Fe1 1_445 . 4_556 130.895(9) ?
Rb1 Rb1 Se1 1_445 . 1_445 47.306(7) ?
Rb1 Rb1 Se1 1_445 . 1_455 90.000(3) ?
Rb1 Rb1 Se1 1_445 . . 132.694(7) ?
Rb1 Rb1 Se1 1_445 . 4_446 47.306(7) ?
Rb1 Rb1 Se1 1_445 . 4_546 90.000(3) ?
Rb1 Rb1 Se1 1_445 . 4_556 132.694(7) ?
Rb1 Rb1 O1 1_445 . 1_445 31.95(5) ?
Rb1 Rb1 O1 1_445 . . 148.05(5) ?
Rb1 Rb1 O1 1_445 . 2_555 66.09(5) ?
Rb1 Rb1 O1 1_445 . 2_655 116.31(5) ?
Rb1 Rb1 O1 1_445 . 3_555 63.69(5) ?
Rb1 Rb1 O1 1_445 . 3_565 113.91(5) ?
Rb1 Rb1 O1 1_445 . 4_446 31.95(5) ?
Rb1 Rb1 O1 1_445 . 4_556 148.05(5) ?
Rb1 Rb1 O1 1_445 . 5_556 66.09(5) ?
Rb1 Rb1 O1 1_445 . 5_566 116.31(5) ?
Rb1 Rb1 O1 1_445 . 6_556 63.69(5) ?
Rb1 Rb1 O1 1_445 . 6_656 113.91(5) ?
Rb1 Rb1 Rb1 1_455 . 1_545 120.000(2) ?
Rb1 Rb1 Rb1 1_455 . 1_565 60.000(2) ?
Rb1 Rb1 Rb1 1_455 . 1_655 180.0(5) ?
Rb1 Rb1 Rb1 1_455 . 1_665 120.000(3) ?
Rb1 Rb1 Fe1 1_455 . 1_445 49.105(9) ?
Rb1 Rb1 Fe1 1_455 . 1_545 130.895(9) ?
Rb1 Rb1 Fe1 1_455 . . 90.000(2) ?
Rb1 Rb1 Fe1 1_455 . 4_446 90.000(2) ?
Rb1 Rb1 Fe1 1_455 . 4_456 49.105(9) ?
Rb1 Rb1 Fe1 1_455 . 4_556 130.895(9) ?
Rb1 Rb1 Se1 1_455 . 1_445 90.000(2) ?
Rb1 Rb1 Se1 1_455 . 1_455 47.306(7) ?
Rb1 Rb1 Se1 1_455 . . 132.694(7) ?
Rb1 Rb1 Se1 1_455 . 4_446 47.306(7) ?
Rb1 Rb1 Se1 1_455 . 4_546 132.694(7) ?
Rb1 Rb1 Se1 1_455 . 4_556 90.000(2) ?
Rb1 Rb1 O1 1_455 . 1_445 66.09(5) ?
Rb1 Rb1 O1 1_455 . . 116.31(5) ?
Rb1 Rb1 O1 1_455 . 2_555 31.95(6) ?
Rb1 Rb1 O1 1_455 . 2_655 148.05(6) ?
Rb1 Rb1 O1 1_455 . 3_555 113.91(6) ?
Rb1 Rb1 O1 1_455 . 3_565 63.69(6) ?
Rb1 Rb1 O1 1_455 . 4_446 63.69(5) ?
Rb1 Rb1 O1 1_455 . 4_556 113.91(5) ?
Rb1 Rb1 O1 1_455 . 5_556 116.31(6) ?
Rb1 Rb1 O1 1_455 . 5_566 66.09(6) ?
Rb1 Rb1 O1 1_455 . 6_556 31.95(6) ?
Rb1 Rb1 O1 1_455 . 6_656 148.05(6) ?
Rb1 Rb1 Rb1 1_545 . 1_565 180.0(5) ?
Rb1 Rb1 Rb1 1_545 . 1_655 60.000(2) ?
Rb1 Rb1 Rb1 1_545 . 1_665 120.000(3) ?
Rb1 Rb1 Fe1 1_545 . 1_445 90.000(2) ?
Rb1 Rb1 Fe1 1_545 . 1_545 49.105(9) ?
Rb1 Rb1 Fe1 1_545 . . 130.895(9) ?
Rb1 Rb1 Fe1 1_545 . 4_446 49.105(9) ?
Rb1 Rb1 Fe1 1_545 . 4_456 130.895(9) ?
Rb1 Rb1 Fe1 1_545 . 4_556 90.000(2) ?
Rb1 Rb1 Se1 1_545 . 1_445 47.306(7) ?
Rb1 Rb1 Se1 1_545 . 1_455 132.694(7) ?
Rb1 Rb1 Se1 1_545 . . 90.000(2) ?
Rb1 Rb1 Se1 1_545 . 4_446 90.000(2) ?
Rb1 Rb1 Se1 1_545 . 4_546 47.306(7) ?
Rb1 Rb1 Se1 1_545 . 4_556 132.694(7) ?
Rb1 Rb1 O1 1_545 . 1_445 63.69(5) ?
Rb1 Rb1 O1 1_545 . . 113.91(5) ?
Rb1 Rb1 O1 1_545 . 2_555 116.31(6) ?
Rb1 Rb1 O1 1_545 . 2_655 66.09(6) ?
Rb1 Rb1 O1 1_545 . 3_555 31.95(6) ?
Rb1 Rb1 O1 1_545 . 3_565 148.05(6) ?
Rb1 Rb1 O1 1_545 . 4_446 66.09(5) ?
Rb1 Rb1 O1 1_545 . 4_556 116.31(5) ?
Rb1 Rb1 O1 1_545 . 5_556 31.95(6) ?
Rb1 Rb1 O1 1_545 . 5_566 148.05(6) ?
Rb1 Rb1 O1 1_545 . 6_556 113.91(6) ?
Rb1 Rb1 O1 1_545 . 6_656 63.69(6) ?
Rb1 Rb1 Rb1 1_565 . 1_655 120.000(2) ?
Rb1 Rb1 Rb1 1_565 . 1_665 60.000(3) ?
Rb1 Rb1 Fe1 1_565 . 1_445 90.000(2) ?
Rb1 Rb1 Fe1 1_565 . 1_545 130.895(9) ?
Rb1 Rb1 Fe1 1_565 . . 49.105(9) ?
Rb1 Rb1 Fe1 1_565 . 4_446 130.895(9) ?
Rb1 Rb1 Fe1 1_565 . 4_456 49.105(9) ?
Rb1 Rb1 Fe1 1_565 . 4_556 90.000(2) ?
Rb1 Rb1 Se1 1_565 . 1_445 132.694(7) ?
Rb1 Rb1 Se1 1_565 . 1_455 47.306(7) ?
Rb1 Rb1 Se1 1_565 . . 90.000(2) ?
Rb1 Rb1 Se1 1_565 . 4_446 90.000(2) ?
Rb1 Rb1 Se1 1_565 . 4_546 132.694(7) ?
Rb1 Rb1 Se1 1_565 . 4_556 47.306(7) ?
Rb1 Rb1 O1 1_565 . 1_445 116.31(5) ?
Rb1 Rb1 O1 1_565 . . 66.09(5) ?
Rb1 Rb1 O1 1_565 . 2_555 63.69(6) ?
Rb1 Rb1 O1 1_565 . 2_655 113.91(6) ?
Rb1 Rb1 O1 1_565 . 3_555 148.05(6) ?
Rb1 Rb1 O1 1_565 . 3_565 31.95(6) ?
Rb1 Rb1 O1 1_565 . 4_446 113.91(5) ?
Rb1 Rb1 O1 1_565 . 4_556 63.69(5) ?
Rb1 Rb1 O1 1_565 . 5_556 148.05(6) ?
Rb1 Rb1 O1 1_565 . 5_566 31.95(6) ?
Rb1 Rb1 O1 1_565 . 6_556 66.09(6) ?
Rb1 Rb1 O1 1_565 . 6_656 116.31(6) ?
Rb1 Rb1 Rb1 1_655 . 1_665 60.000(3) ?
Rb1 Rb1 Fe1 1_655 . 1_445 130.895(9) ?
Rb1 Rb1 Fe1 1_655 . 1_545 49.105(9) ?
Rb1 Rb1 Fe1 1_655 . . 90.000(2) ?
Rb1 Rb1 Fe1 1_655 . 4_446 90.000(2) ?
Rb1 Rb1 Fe1 1_655 . 4_456 130.895(9) ?
Rb1 Rb1 Fe1 1_655 . 4_556 49.105(9) ?
Rb1 Rb1 Se1 1_655 . 1_445 90.000(2) ?
Rb1 Rb1 Se1 1_655 . 1_455 132.694(7) ?
Rb1 Rb1 Se1 1_655 . . 47.306(7) ?
Rb1 Rb1 Se1 1_655 . 4_446 132.694(7) ?
Rb1 Rb1 Se1 1_655 . 4_546 47.306(7) ?
Rb1 Rb1 Se1 1_655 . 4_556 90.000(2) ?
Rb1 Rb1 O1 1_655 . 1_445 113.91(5) ?
Rb1 Rb1 O1 1_655 . . 63.69(5) ?
Rb1 Rb1 O1 1_655 . 2_555 148.05(6) ?
Rb1 Rb1 O1 1_655 . 2_655 31.95(6) ?
Rb1 Rb1 O1 1_655 . 3_555 66.09(6) ?
Rb1 Rb1 O1 1_655 . 3_565 116.31(6) ?
Rb1 Rb1 O1 1_655 . 4_446 116.31(5) ?
Rb1 Rb1 O1 1_655 . 4_556 66.09(5) ?
Rb1 Rb1 O1 1_655 . 5_556 63.69(6) ?
Rb1 Rb1 O1 1_655 . 5_566 113.91(6) ?
Rb1 Rb1 O1 1_655 . 6_556 148.05(6) ?
Rb1 Rb1 O1 1_655 . 6_656 31.95(6) ?
Rb1 Rb1 Fe1 1_665 . 1_445 130.895(9) ?
Rb1 Rb1 Fe1 1_665 . 1_545 90.000(3) ?
Rb1 Rb1 Fe1 1_665 . . 49.105(9) ?
Rb1 Rb1 Fe1 1_665 . 4_446 130.895(9) ?
Rb1 Rb1 Fe1 1_665 . 4_456 90.000(3) ?
Rb1 Rb1 Fe1 1_665 . 4_556 49.105(9) ?
Rb1 Rb1 Se1 1_665 . 1_445 132.694(7) ?
Rb1 Rb1 Se1 1_665 . 1_455 90.000(3) ?
Rb1 Rb1 Se1 1_665 . . 47.306(7) ?
Rb1 Rb1 Se1 1_665 . 4_446 132.694(7) ?
Rb1 Rb1 Se1 1_665 . 4_546 90.000(3) ?
Rb1 Rb1 Se1 1_665 . 4_556 47.306(7) ?
Rb1 Rb1 O1 1_665 . 1_445 148.05(5) ?
Rb1 Rb1 O1 1_665 . . 31.95(5) ?
Rb1 Rb1 O1 1_665 . 2_555 113.91(5) ?
Rb1 Rb1 O1 1_665 . 2_655 63.69(5) ?
Rb1 Rb1 O1 1_665 . 3_555 116.31(5) ?
Rb1 Rb1 O1 1_665 . 3_565 66.09(5) ?
Rb1 Rb1 O1 1_665 . 4_446 148.05(5) ?
Rb1 Rb1 O1 1_665 . 4_556 31.95(5) ?
Rb1 Rb1 O1 1_665 . 5_556 113.91(5) ?
Rb1 Rb1 O1 1_665 . 5_566 63.69(5) ?
Rb1 Rb1 O1 1_665 . 6_556 116.31(5) ?
Rb1 Rb1 O1 1_665 . 6_656 66.09(5) ?
Fe1 Rb1 Fe1 1_445 . 1_545 81.790(13) ?
Fe1 Rb1 Fe1 1_445 . . 81.790(13) ?
Fe1 Rb1 Fe1 1_445 . 4_446 98.210(13) ?
Fe1 Rb1 Fe1 1_445 . 4_456 98.210(13) ?
Fe1 Rb1 Fe1 1_445 . 4_556 180.0(5) ?
Fe1 Rb1 Se1 1_445 . 1_445 45.320(5) ?
Fe1 Rb1 Se1 1_445 . 1_455 45.319(6) ?
Fe1 Rb1 Se1 1_445 . . 100.644(15) ?
Fe1 Rb1 Se1 1_445 . 4_446 79.356(15) ?
Fe1 Rb1 Se1 1_445 . 4_546 134.681(6) ?
Fe1 Rb1 Se1 1_445 . 4_556 134.680(5) ?
Fe1 Rb1 O1 1_445 . 1_445 26.70(5) ?
Fe1 Rb1 O1 1_445 . . 102.57(5) ?
Fe1 Rb1 O1 1_445 . 2_555 26.70(6) ?
Fe1 Rb1 O1 1_445 . 2_655 102.57(5) ?
Fe1 Rb1 O1 1_445 . 3_555 68.74(6) ?
Fe1 Rb1 O1 1_445 . 3_565 68.74(5) ?
Fe1 Rb1 O1 1_445 . 4_446 77.43(5) ?
Fe1 Rb1 O1 1_445 . 4_556 153.30(5) ?
Fe1 Rb1 O1 1_445 . 5_556 111.26(5) ?
Fe1 Rb1 O1 1_445 . 5_566 111.26(6) ?
Fe1 Rb1 O1 1_445 . 6_556 77.43(5) ?
Fe1 Rb1 O1 1_445 . 6_656 153.30(6) ?
Fe1 Rb1 Fe1 1_545 . . 81.790(13) ?
Fe1 Rb1 Fe1 1_545 . 4_446 98.210(13) ?
Fe1 Rb1 Fe1 1_545 . 4_456 180.0(5) ?
Fe1 Rb1 Fe1 1_545 . 4_556 98.210(13) ?
Fe1 Rb1 Se1 1_545 . 1_445 45.319(6) ?
Fe1 Rb1 Se1 1_545 . 1_455 100.643(15) ?
Fe1 Rb1 Se1 1_545 . . 45.319(6) ?
Fe1 Rb1 Se1 1_545 . 4_446 134.681(6) ?
Fe1 Rb1 Se1 1_545 . 4_546 79.357(15) ?
Fe1 Rb1 Se1 1_545 . 4_556 134.681(6) ?
Fe1 Rb1 O1 1_545 . 1_445 68.74(5) ?
Fe1 Rb1 O1 1_545 . . 68.74(5) ?
Fe1 Rb1 O1 1_545 . 2_555 102.57(6) ?
Fe1 Rb1 O1 1_545 . 2_655 26.70(5) ?
Fe1 Rb1 O1 1_545 . 3_555 26.70(5) ?
Fe1 Rb1 O1 1_545 . 3_565 102.57(6) ?
Fe1 Rb1 O1 1_545 . 4_446 111.26(5) ?
Fe1 Rb1 O1 1_545 . 4_556 111.26(5) ?
Fe1 Rb1 O1 1_545 . 5_556 77.43(6) ?
Fe1 Rb1 O1 1_545 . 5_566 153.30(5) ?
Fe1 Rb1 O1 1_545 . 6_556 153.30(5) ?
Fe1 Rb1 O1 1_545 . 6_656 77.43(6) ?
Fe1 Rb1 Fe1 . . 4_446 180.0(5) ?
Fe1 Rb1 Fe1 . . 4_456 98.210(13) ?
Fe1 Rb1 Fe1 . . 4_556 98.210(13) ?
Fe1 Rb1 Se1 . . 1_445 100.644(15) ?
Fe1 Rb1 Se1 . . 1_455 45.319(6) ?
Fe1 Rb1 Se1 . . . 45.320(5) ?
Fe1 Rb1 Se1 . . 4_446 134.680(5) ?
Fe1 Rb1 Se1 . . 4_546 134.681(6) ?
Fe1 Rb1 Se1 . . 4_556 79.356(15) ?
Fe1 Rb1 O1 . . 1_445 102.57(5) ?
Fe1 Rb1 O1 . . . 26.70(5) ?
Fe1 Rb1 O1 . . 2_555 68.74(5) ?
Fe1 Rb1 O1 . . 2_655 68.74(6) ?
Fe1 Rb1 O1 . . 3_555 102.57(5) ?
Fe1 Rb1 O1 . . 3_565 26.70(6) ?
Fe1 Rb1 O1 . . 4_446 153.30(5) ?
Fe1 Rb1 O1 . . 4_556 77.43(5) ?
Fe1 Rb1 O1 . . 5_556 153.30(6) ?
Fe1 Rb1 O1 . . 5_566 77.43(5) ?
Fe1 Rb1 O1 . . 6_556 111.26(6) ?
Fe1 Rb1 O1 . . 6_656 111.26(5) ?
Fe1 Rb1 Fe1 4_446 . 4_456 81.790(13) ?
Fe1 Rb1 Fe1 4_446 . 4_556 81.790(13) ?
Fe1 Rb1 Se1 4_446 . 1_445 79.356(15) ?
Fe1 Rb1 Se1 4_446 . 1_455 134.681(6) ?
Fe1 Rb1 Se1 4_446 . . 134.680(5) ?
Fe1 Rb1 Se1 4_446 . 4_446 45.320(5) ?
Fe1 Rb1 Se1 4_446 . 4_546 45.319(6) ?
Fe1 Rb1 Se1 4_446 . 4_556 100.644(15) ?
Fe1 Rb1 O1 4_446 . 1_445 77.43(5) ?
Fe1 Rb1 O1 4_446 . . 153.30(5) ?
Fe1 Rb1 O1 4_446 . 2_555 111.26(5) ?
Fe1 Rb1 O1 4_446 . 2_655 111.26(6) ?
Fe1 Rb1 O1 4_446 . 3_555 77.43(5) ?
Fe1 Rb1 O1 4_446 . 3_565 153.30(6) ?
Fe1 Rb1 O1 4_446 . 4_446 26.70(5) ?
Fe1 Rb1 O1 4_446 . 4_556 102.57(5) ?
Fe1 Rb1 O1 4_446 . 5_556 26.70(6) ?
Fe1 Rb1 O1 4_446 . 5_566 102.57(5) ?
Fe1 Rb1 O1 4_446 . 6_556 68.74(6) ?
Fe1 Rb1 O1 4_446 . 6_656 68.74(5) ?
Fe1 Rb1 Fe1 4_456 . 4_556 81.790(13) ?
Fe1 Rb1 Se1 4_456 . 1_445 134.681(6) ?
Fe1 Rb1 Se1 4_456 . 1_455 79.357(15) ?
Fe1 Rb1 Se1 4_456 . . 134.681(6) ?
Fe1 Rb1 Se1 4_456 . 4_446 45.319(6) ?
Fe1 Rb1 Se1 4_456 . 4_546 100.643(15) ?
Fe1 Rb1 Se1 4_456 . 4_556 45.319(6) ?
Fe1 Rb1 O1 4_456 . 1_445 111.26(5) ?
Fe1 Rb1 O1 4_456 . . 111.26(5) ?
Fe1 Rb1 O1 4_456 . 2_555 77.43(6) ?
Fe1 Rb1 O1 4_456 . 2_655 153.30(5) ?
Fe1 Rb1 O1 4_456 . 3_555 153.30(5) ?
Fe1 Rb1 O1 4_456 . 3_565 77.43(6) ?
Fe1 Rb1 O1 4_456 . 4_446 68.74(5) ?
Fe1 Rb1 O1 4_456 . 4_556 68.74(5) ?
Fe1 Rb1 O1 4_456 . 5_556 102.57(6) ?
Fe1 Rb1 O1 4_456 . 5_566 26.70(5) ?
Fe1 Rb1 O1 4_456 . 6_556 26.70(5) ?
Fe1 Rb1 O1 4_456 . 6_656 102.57(6) ?
Fe1 Rb1 Se1 4_556 . 1_445 134.680(5) ?
Fe1 Rb1 Se1 4_556 . 1_455 134.681(6) ?
Fe1 Rb1 Se1 4_556 . . 79.356(15) ?
Fe1 Rb1 Se1 4_556 . 4_446 100.644(15) ?
Fe1 Rb1 Se1 4_556 . 4_546 45.319(6) ?
Fe1 Rb1 Se1 4_556 . 4_556 45.320(5) ?
Fe1 Rb1 O1 4_556 . 1_445 153.30(5) ?
Fe1 Rb1 O1 4_556 . . 77.43(5) ?
Fe1 Rb1 O1 4_556 . 2_555 153.30(6) ?
Fe1 Rb1 O1 4_556 . 2_655 77.43(5) ?
Fe1 Rb1 O1 4_556 . 3_555 111.26(6) ?
Fe1 Rb1 O1 4_556 . 3_565 111.26(5) ?
Fe1 Rb1 O1 4_556 . 4_446 102.57(5) ?
Fe1 Rb1 O1 4_556 . 4_556 26.70(5) ?
Fe1 Rb1 O1 4_556 . 5_556 68.74(5) ?
Fe1 Rb1 O1 4_556 . 5_566 68.74(6) ?
Fe1 Rb1 O1 4_556 . 6_556 102.57(5) ?
Fe1 Rb1 O1 4_556 . 6_656 26.70(6) ?
Se1 Rb1 Se1 1_445 . 1_455 85.388(10) ?
Se1 Rb1 Se1 1_445 . . 85.388(10) ?
Se1 Rb1 Se1 1_445 . 4_446 94.612(10) ?
Se1 Rb1 Se1 1_445 . 4_546 94.612(10) ?
Se1 Rb1 Se1 1_445 . 4_556 180.0(5) ?
Se1 Rb1 O1 1_445 . 1_445 24.10(5) ?
Se1 Rb1 O1 1_445 . . 103.77(5) ?
Se1 Rb1 O1 1_445 . 2_555 71.84(6) ?
Se1 Rb1 O1 1_445 . 2_655 71.84(5) ?
Se1 Rb1 O1 1_445 . 3_555 24.10(6) ?
Se1 Rb1 O1 1_445 . 3_565 103.77(5) ?
Se1 Rb1 O1 1_445 . 4_446 76.23(5) ?
Se1 Rb1 O1 1_445 . 4_556 155.90(5) ?
Se1 Rb1 O1 1_445 . 5_556 76.23(5) ?
Se1 Rb1 O1 1_445 . 5_566 155.90(6) ?
Se1 Rb1 O1 1_445 . 6_556 108.16(5) ?
Se1 Rb1 O1 1_445 . 6_656 108.16(6) ?
Se1 Rb1 Se1 1_455 . . 85.388(10) ?
Se1 Rb1 Se1 1_455 . 4_446 94.612(10) ?
Se1 Rb1 Se1 1_455 . 4_546 180.0(5) ?
Se1 Rb1 Se1 1_455 . 4_556 94.612(10) ?
Se1 Rb1 O1 1_455 . 1_445 71.84(5) ?
Se1 Rb1 O1 1_455 . . 71.84(5) ?
Se1 Rb1 O1 1_455 . 2_555 24.10(5) ?
Se1 Rb1 O1 1_455 . 2_655 103.77(6) ?
Se1 Rb1 O1 1_455 . 3_555 103.77(6) ?
Se1 Rb1 O1 1_455 . 3_565 24.10(5) ?
Se1 Rb1 O1 1_455 . 4_446 108.16(5) ?
Se1 Rb1 O1 1_455 . 4_556 108.16(5) ?
Se1 Rb1 O1 1_455 . 5_556 155.90(5) ?
Se1 Rb1 O1 1_455 . 5_566 76.23(6) ?
Se1 Rb1 O1 1_455 . 6_556 76.23(6) ?
Se1 Rb1 O1 1_455 . 6_656 155.90(5) ?
Se1 Rb1 Se1 . . 4_446 180.0(5) ?
Se1 Rb1 Se1 . . 4_546 94.612(10) ?
Se1 Rb1 Se1 . . 4_556 94.612(10) ?
Se1 Rb1 O1 . . 1_445 103.77(5) ?
Se1 Rb1 O1 . . . 24.10(5) ?
Se1 Rb1 O1 . . 2_555 103.77(5) ?
Se1 Rb1 O1 . . 2_655 24.10(6) ?
Se1 Rb1 O1 . . 3_555 71.84(5) ?
Se1 Rb1 O1 . . 3_565 71.84(6) ?
Se1 Rb1 O1 . . 4_446 155.90(5) ?
Se1 Rb1 O1 . . 4_556 76.23(5) ?
Se1 Rb1 O1 . . 5_556 108.16(6) ?
Se1 Rb1 O1 . . 5_566 108.16(5) ?
Se1 Rb1 O1 . . 6_556 155.90(6) ?
Se1 Rb1 O1 . . 6_656 76.23(5) ?
Se1 Rb1 Se1 4_446 . 4_546 85.388(10) ?
Se1 Rb1 Se1 4_446 . 4_556 85.388(10) ?
Se1 Rb1 O1 4_446 . 1_445 76.23(5) ?
Se1 Rb1 O1 4_446 . . 155.90(5) ?
Se1 Rb1 O1 4_446 . 2_555 76.23(5) ?
Se1 Rb1 O1 4_446 . 2_655 155.90(6) ?
Se1 Rb1 O1 4_446 . 3_555 108.16(5) ?
Se1 Rb1 O1 4_446 . 3_565 108.16(6) ?
Se1 Rb1 O1 4_446 . 4_446 24.10(5) ?
Se1 Rb1 O1 4_446 . 4_556 103.77(5) ?
Se1 Rb1 O1 4_446 . 5_556 71.84(6) ?
Se1 Rb1 O1 4_446 . 5_566 71.84(5) ?
Se1 Rb1 O1 4_446 . 6_556 24.10(6) ?
Se1 Rb1 O1 4_446 . 6_656 103.77(5) ?
Se1 Rb1 Se1 4_546 . 4_556 85.388(10) ?
Se1 Rb1 O1 4_546 . 1_445 108.16(5) ?
Se1 Rb1 O1 4_546 . . 108.16(5) ?
Se1 Rb1 O1 4_546 . 2_555 155.90(5) ?
Se1 Rb1 O1 4_546 . 2_655 76.23(6) ?
Se1 Rb1 O1 4_546 . 3_555 76.23(6) ?
Se1 Rb1 O1 4_546 . 3_565 155.90(5) ?
Se1 Rb1 O1 4_546 . 4_446 71.84(5) ?
Se1 Rb1 O1 4_546 . 4_556 71.84(5) ?
Se1 Rb1 O1 4_546 . 5_556 24.10(5) ?
Se1 Rb1 O1 4_546 . 5_566 103.77(6) ?
Se1 Rb1 O1 4_546 . 6_556 103.77(6) ?
Se1 Rb1 O1 4_546 . 6_656 24.10(5) ?
Se1 Rb1 O1 4_556 . 1_445 155.90(5) ?
Se1 Rb1 O1 4_556 . . 76.23(5) ?
Se1 Rb1 O1 4_556 . 2_555 108.16(6) ?
Se1 Rb1 O1 4_556 . 2_655 108.16(5) ?
Se1 Rb1 O1 4_556 . 3_555 155.90(6) ?
Se1 Rb1 O1 4_556 . 3_565 76.23(5) ?
Se1 Rb1 O1 4_556 . 4_446 103.77(5) ?
Se1 Rb1 O1 4_556 . 4_556 24.10(5) ?
Se1 Rb1 O1 4_556 . 5_556 103.77(5) ?
Se1 Rb1 O1 4_556 . 5_566 24.10(6) ?
Se1 Rb1 O1 4_556 . 6_556 71.84(5) ?
Se1 Rb1 O1 4_556 . 6_656 71.84(6) ?
O1 Rb1 O1 1_445 . . 116.11(7) ?
O1 Rb1 O1 1_445 . 2_555 52.62(8) ?
O1 Rb1 O1 1_445 . 2_655 94.63(7) ?
O1 Rb1 O1 1_445 . 3_555 47.82(8) ?
O1 Rb1 O1 1_445 . 3_565 94.63(7) ?
O1 Rb1 O1 1_445 . 4_446 63.89(7) ?
O1 Rb1 O1 1_445 . 4_556 180.0(5) ?
O1 Rb1 O1 1_445 . 5_556 85.37(7) ?
O1 Rb1 O1 1_445 . 5_566 132.18(8) ?
O1 Rb1 O1 1_445 . 6_556 85.37(7) ?
O1 Rb1 O1 1_445 . 6_656 127.38(8) ?
O1 Rb1 O1 . . 2_555 94.63(7) ?
O1 Rb1 O1 . . 2_655 47.82(8) ?
O1 Rb1 O1 . . 3_555 94.63(7) ?
O1 Rb1 O1 . . 3_565 52.62(8) ?
O1 Rb1 O1 . . 4_446 180.0(5) ?
O1 Rb1 O1 . . 4_556 63.89(7) ?
O1 Rb1 O1 . . 5_556 127.38(8) ?
O1 Rb1 O1 . . 5_566 85.37(7) ?
O1 Rb1 O1 . . 6_556 132.18(8) ?
O1 Rb1 O1 . . 6_656 85.37(7) ?
O1 Rb1 O1 2_555 . 2_655 116.11(8) ?
O1 Rb1 O1 2_555 . 3_555 94.63(9) ?
O1 Rb1 O1 2_555 . 3_565 47.82(7) ?
O1 Rb1 O1 2_555 . 4_446 85.37(7) ?
O1 Rb1 O1 2_555 . 4_556 127.38(8) ?
O1 Rb1 O1 2_555 . 5_556 132.18(7) ?
O1 Rb1 O1 2_555 . 5_566 85.37(9) ?
O1 Rb1 O1 2_555 . 6_556 63.89(8) ?
O1 Rb1 O1 2_555 . 6_656 180.0(5) ?
O1 Rb1 O1 2_655 . 3_555 52.62(7) ?
O1 Rb1 O1 2_655 . 3_565 94.63(9) ?
O1 Rb1 O1 2_655 . 4_446 132.18(8) ?
O1 Rb1 O1 2_655 . 4_556 85.37(7) ?
O1 Rb1 O1 2_655 . 5_556 85.37(9) ?
O1 Rb1 O1 2_655 . 5_566 127.38(7) ?
O1 Rb1 O1 2_655 . 6_556 180.0(5) ?
O1 Rb1 O1 2_655 . 6_656 63.89(8) ?
O1 Rb1 O1 3_555 . 3_565 116.11(8) ?
O1 Rb1 O1 3_555 . 4_446 85.37(7) ?
O1 Rb1 O1 3_555 . 4_556 132.18(8) ?
O1 Rb1 O1 3_555 . 5_556 63.89(8) ?
O1 Rb1 O1 3_555 . 5_566 180.0(5) ?
O1 Rb1 O1 3_555 . 6_556 127.38(7) ?
O1 Rb1 O1 3_555 . 6_656 85.37(9) ?
O1 Rb1 O1 3_565 . 4_446 127.38(8) ?
O1 Rb1 O1 3_565 . 4_556 85.37(7) ?
O1 Rb1 O1 3_565 . 5_556 180.0(5) ?
O1 Rb1 O1 3_565 . 5_566 63.89(8) ?
O1 Rb1 O1 3_565 . 6_556 85.37(9) ?
O1 Rb1 O1 3_565 . 6_656 132.18(7) ?
O1 Rb1 O1 4_446 . 4_556 116.11(7) ?
O1 Rb1 O1 4_446 . 5_556 52.62(8) ?
O1 Rb1 O1 4_446 . 5_566 94.63(7) ?
O1 Rb1 O1 4_446 . 6_556 47.82(8) ?
O1 Rb1 O1 4_446 . 6_656 94.63(7) ?
O1 Rb1 O1 4_556 . 5_556 94.63(7) ?
O1 Rb1 O1 4_556 . 5_566 47.82(8) ?
O1 Rb1 O1 4_556 . 6_556 94.63(7) ?
O1 Rb1 O1 4_556 . 6_656 52.62(8) ?
O1 Rb1 O1 5_556 . 5_566 116.11(8) ?
O1 Rb1 O1 5_556 . 6_556 94.63(9) ?
O1 Rb1 O1 5_556 . 6_656 47.82(7) ?
O1 Rb1 O1 5_566 . 6_556 52.62(7) ?
O1 Rb1 O1 5_566 . 6_656 94.63(9) ?
O1 Rb1 O1 6_556 . 6_656 116.11(8) ?
Rb1 Fe1 Rb1 . . 1_565 81.790(18) ?
Rb1 Fe1 Rb1 . . 1_665 81.790(18) ?
Rb1 Fe1 F1 . . . 79.34(9) ?
Rb1 Fe1 F1 . . 2_665 134.67(14) ?
Rb1 Fe1 F1 . . 3_565 134.67(9) ?
Rb1 Fe1 O1 . . . 48.13(7) ?
Rb1 Fe1 O1 . . 2_665 107.11(10) ?
Rb1 Fe1 O1 . . 3_565 48.13(10) ?
Rb1 Fe1 Rb1 1_565 . 1_665 81.790(18) ?
Rb1 Fe1 F1 1_565 . . 134.67(6) ?
Rb1 Fe1 F1 1_565 . 2_665 134.67(12) ?
Rb1 Fe1 F1 1_565 . 3_565 79.34(10) ?
Rb1 Fe1 O1 1_565 . . 107.11(10) ?
Rb1 Fe1 O1 1_565 . 2_665 48.13(8) ?
Rb1 Fe1 O1 1_565 . 3_565 48.13(8) ?
Rb1 Fe1 F1 1_665 . . 134.67(9) ?
Rb1 Fe1 F1 1_665 . 2_665 79.34(9) ?
Rb1 Fe1 F1 1_665 . 3_565 134.67(5) ?
Rb1 Fe1 O1 1_665 . . 48.13(7) ?
Rb1 Fe1 O1 1_665 . 2_665 48.13(10) ?
Rb1 Fe1 O1 1_665 . 3_565 107.11(10) ?
F1 Fe1 F1 . . 2_665 85.42(12) ?
F1 Fe1 F1 . . 3_565 85.42(12) ?
F1 Fe1 O1 . . . 89.85(13) ?
F1 Fe1 O1 . . 2_665 173.56(14) ?
F1 Fe1 O1 . . 3_565 89.85(10) ?
F1 Fe1 F1 2_665 . 3_565 85.42(17) ?
F1 Fe1 O1 2_665 . . 89.85(15) ?
F1 Fe1 O1 2_665 . 2_665 89.85(13) ?
F1 Fe1 O1 2_665 . 3_565 173.56(14) ?
F1 Fe1 O1 3_565 . . 173.56(15) ?
F1 Fe1 O1 3_565 . 2_665 89.85(12) ?
F1 Fe1 O1 3_565 . 3_565 89.85(15) ?
O1 Fe1 O1 . . 2_665 94.52(13) ?
O1 Fe1 O1 . . 3_565 94.52(13) ?
O1 Fe1 O1 2_665 . 3_565 94.52(12) ?
F1 Fe2 F1 . . 2_555 90.18(12) ?
F1 Fe2 F1 . . 3_555 90.18(12) ?
F1 Fe2 F1 . . 4_555 89.82(9) ?
F1 Fe2 F1 . . 5_555 180.0(5) ?
F1 Fe2 F1 . . 6_555 89.82(15) ?
F1 Fe2 F1 2_555 . 3_555 90.18(17) ?
F1 Fe2 F1 2_555 . 4_555 180.0(5) ?
F1 Fe2 F1 2_555 . 5_555 89.82(15) ?
F1 Fe2 F1 2_555 . 6_555 89.82(15) ?
F1 Fe2 F1 3_555 . 4_555 89.82(15) ?
F1 Fe2 F1 3_555 . 5_555 89.82(15) ?
F1 Fe2 F1 3_555 . 6_555 180.0(5) ?
F1 Fe2 F1 4_555 . 5_555 90.18(12) ?
F1 Fe2 F1 4_555 . 6_555 90.18(12) ?
F1 Fe2 F1 5_555 . 6_555 90.18(17) ?
Rb1 Se1 Rb1 . . 1_655 85.388(14) ?
Rb1 Se1 Rb1 . . 1_665 85.388(14) ?
Rb1 Se1 O1 . . . 50.34(7) ?
Rb1 Se1 O1 . . 2_655 50.34(11) ?
Rb1 Se1 O1 . . 3_665 113.45(11) ?
Rb1 Se1 Rb1 1_655 . 1_665 85.388(14) ?
Rb1 Se1 O1 1_655 . . 113.45(11) ?
Rb1 Se1 O1 1_655 . 2_655 50.34(9) ?
Rb1 Se1 O1 1_655 . 3_665 50.34(9) ?
Rb1 Se1 O1 1_665 . . 50.34(7) ?
Rb1 Se1 O1 1_665 . 2_655 113.45(11) ?
Rb1 Se1 O1 1_665 . 3_665 50.34(11) ?
O1 Se1 O1 . . 2_655 99.65(15) ?
O1 Se1 O1 . . 3_665 99.65(15) ?
O1 Se1 O1 2_655 . 3_665 99.65(13) ?
Fe1 F1 Fe2 . . . 176.69(18) ?
Rb1 O1 Rb1 . . 1_665 116.11(10) ?
Rb1 O1 Fe1 . . . 105.17(9) ?
Rb1 O1 Se1 . . . 105.56(10) ?
Rb1 O1 Fe1 1_665 . . 105.17(9) ?
Rb1 O1 Se1 1_665 . . 105.56(10) ?
Fe1 O1 Se1 . . . 119.92(18) ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?


